### A micromechanical fracture analysis to investigate the effect of healing particles on the

### overall mechanical response of a self-healing particulate composite

Ponnusami, Sathiskumar A.; Krishnasamy, Jayaprakash; Turteltaub, Sergio; van der Zwaag, Sybrand DOI

10.1111/ffe.12929

Publication date 2019

Document Version Final published version Published in

Fatigue and Fracture of Engineering Materials and Structures

Citation (APA)

Ponnusami, S. A., Krishnasamy, J., Turteltaub, S., & van der Zwaag, S. (2019). A micromechanical fracture analysis to investigate the effect of healing particles on the overall mechanical response of a self-healing particulate composite. Fatigue and Fracture of Engineering Materials and Structures, 42(2), 533-545. https://doi.org/10.1111/ffe.12929

Important note

To cite this publication, please use the final published version (if applicable). Please check the document version above.

Copyright

Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons. Takedown policy

Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.

This work is downloaded from Delft University of Technology.

DOI: 10.1111/ffe.12929

**O R I G I N A L C O N T R I B U T I O N**

**A micromechanical fracture analysis to investigate the**

**effect of healing particles on the overall mechanical**

**response of a self-healing particulate composite**

### Sathiskumar A. Ponnusami

1,2_{Jayaprakash Krishnasamy}

1 _{Sergio Turteltaub}

1
### Sybrand van der Zwaag

11_{Faculty of Aerospace Engineering, Delft}

University of Technology, Delft, The Netherlands

2_{Solid Mechanics and Materials}

Engineering, Department of Engineering Science, University of Oxford, Oxford, UK

**Correspondence**

Sathiskumar A. Ponnusami, Faculty of Aerospace Engineering, Delft University of Technology, Kluyverweg 1, 2629 HS, Delft, The Netherlands.

Email: [email protected]

**Funding information**

Dutch Government's IOP Self Healing Materials , Grant/Award Number: SHM01021 ; European Union's seventh framework program (FP7) - NMP SAMBA project , Grant/Award Number: 309849

**ABSTRACT**

A computational fracture analysis is conducted on a self-healing particulate composite employing a finite element model of an actual microstructure. The key objective is to quantify the effects of the actual morphology and the fracture properties of the healing particles on the overall mechanical behaviour of the (MoSi2) particle-dispersed Yttria Stabilised Zirconia (YSZ) composite. To simulate fracture, a cohesive zone approach is utilised whereby cohesive elements are embedded throughout the finite element mesh allowing for arbitrary crack initiation and propagation in the microstructure. The fracture behaviour in terms of the composite strength and the percentage of fractured particles is reported as a function of the mismatch in fracture properties between the healing particles and the matrix as well as a function of particle/matrix interface strength and fracture energy. The study can be used as a guiding tool for designing an extrinsic self-healing material and understanding the effect of the healing particles on the overall mechanical properties of the material.

**K E Y WO R D S**

cohesive elements, fracture mechanism, fracture properties, healing particles, self-healing material, thermal barrier coatings

**1**

**I N T RO D U CT I O N**

Self-healing materials can be classified into two broad classes, extrinsic and intrinsic, depending upon the healing mechanism and the healing agent involved. In an intrinsic self-healing material, the healing agent is contained within the host material as its integral constituent. In other words, the healing action is due to the physiochemical nature of the material itself.1

When damage or cracking occurs, one or more con-stituents of the material act as the healing agent,

which upon completion of the healing process aid in
the recovery of the mechanical properties. Such intrinsic
self-healing mechanisms can be found in several material
classes that include ceramics,2,3 _{cementitious materials,}4

and polymers.5 _{In the second class of self-healing }

mate-rials, the extrinsic ones, the healing agent is not part
of the original material itself, rather a discrete foreign
material constituent is added to the host material
dur-ing the fabrication process.6-11 _{This class has been a}

popular approach in the early stages of the field of
self-healing materials development as it favours
*incor-Fatigue Fract Eng Mater Struct***. 2019;42:533–545.** wileyonlinelibrary.com/journal/ffe © 2018 Wiley Publishing Ltd. **533**

porating healing mechanism into any class of material
system that does not inherently possess a self-healing
characteristic. One of the widely used techniques under
this category is encapsulation of the healing agent and
dispersing the healing capsules within the host
mate-rial. When a crack appears in such a material, it
inter-acts with the healing capsule, followed by its rupture or
fracturing.12-15 _{Upon opening of the capsule, the healing}

agent flows or diffuses into the crack eventually leading to crack filling. Such a healing process involves a sequence of steps starting from crack-capsule interaction, rupture of the capsule, followed by the release of the healing agent into the crack, and finally formation of the heal-ing product through a chemical or a physical reaction. The resulting healing product, in turn, binds the crack faces together and restores the mechanical integrity of the material.

From the perspective of (extrinsic) self-healing material design, the properties of the healing particles in relation to the host matrix are very crucial for successful realisa-tion of a self-healing material system. In particular, for the selection and design of healing capsules, the follow-ing two requirements have to be met to result in an ideal self-healing material design:

**• In order to enable activation of the healing process, the**

microcracks in the matrix material should get attracted towards the healing particles and break them, instead of deflecting away from the particles that would prevent healing activation.

**• The introduction of healing particles into the**

matrix should not deteriorate the mechanical prop-erties of the host matrix material. In other words, the structural integrity of the material should not be compromised with the dispersion of the healing particles.

The above two requirements are often contradictory
as promoting particle fracture for healing is likely to
degrade the composite strength, in general. Hence, for
an optimal design of the self-healing material, a
bal-ance between these two requirements has to be achieved.
This, in turn, lies in a careful selection and design of
the healing particles in terms of their geometric and
material properties and their spatial distribution. The
first requirement is dealt in detail,16 _{whereby fracture}

maps distinguishing the fracture mechanisms are gen-erated through extensive two-dimensional analyses on a single-particle matrix system. In this current work, the primary objective is to address the second requirement, whereby microstructure-based two-dimensional finite ele-ment fracture simulations are conducted for the quantifi-cation of the effect of healing capsules on the mechanical properties.

Microstructure-based finite element simulations have
been conducted in the literature to analyse fracture and
damage in particulate composite systems.17-25 _{For }

exam-ples, microstructures representing a random
distribu-tion of irregularly shaped SiC particles in an aluminum
matrix were simulated using two-dimensional linear
elas-tic approach involving stress intensity factor as the crack
driving force parameter.17,18_{The effect of particle }

cluster-ing was quantified, and the resultcluster-ing crack paths were
compared with experiments. In a different work,19 _{an}

actual microstructure of a particulate composite was
mod-elled by mapping the scanning electron microscope (SEM)
images onto the finite element mesh. They investigated the
effects of pore defects and residual stresses on the crack
path by employing Griffith energy-based fracture
mechan-ics approach. An elastoplastic finite element analysis was
conducted on an SEM-based finite element model, and
the stress-strain response was reported as a function of
microstructural features such as particle clustering.20 _{A}

comprehensive investigation of the effect of distribution,
size, and shape of the particulate reinforcements and
inter-phase properties on the fracture behaviour of a Al2O3/TiB2
composite has been conducted.23,24_{Employing a J-integral}

concept and using a cohesive zone approach to simulate
fracture in the matrix, the particle, or the interface, the
effective fracture toughness of the composite was
quan-tified. The abovementioned analyses were performed in
a two-dimensional framework. Some efforts have been
taken to conduct three-dimensional crack propagation
analysis in particulate composites,26-28 _{but the }

computa-tional cost associated with such simulations limits the scope of such studies in terms of number of particles that can be analysed. Further, the computational intensity pre-vents the possibility of conducting a series of parametric analysis to explore the effect of microstructural features and the influence of constituent properties.

In the context of self-healing particulate composite
systems, a limited number of modelling studies have
been conducted in terms of quantifying the effective
mechanical properties and crack path predictions.28-33_{For}

instance, efforts are taken to estimate the effective elastic
properties of self-healing particulate composites, whereby
the effect of dispersed healing particles on the elastic
mod-uli of the host matrix material is quantified.30,31_{Crack }

prop-agation studies were conducted in an idealised healing
capsule(s)-matrix system, and the effects of geometric and
material parameters were analysed using cohesive zone
model and extended finite element method (XFEM).28_{In}

particular, a self-healing concrete in a three-point bend-ing test set-up was utilised to evaluate the influence of parameters such as number, size, and position of capsules on the mechanical behaviour of the concrete. This was then followed by modelling an idealised single healing

capsule-matrix volume element, whereby the influence of interface properties and capsule volume fraction on the effective strength was reported. Nonetheless, for fur-ther material development, it is important to determine the expected performance under actual conditions. Cor-respondingly, the objective of the present research is to study the crack propagation in a real microstructure of a self-healing particulate composite, followed by the quan-tification of the effect of the healing particles and their properties on the composite mechanical behaviour. This is achieved through numerical analysis using a finite ele-ment model generated directly from an actual microstruc-ture of the MoSi2-YSZ composite.34 The motivation is to reveal the roles of these parameters to experimental researchers, which could be helpful in the design and development of self-healing systems with least compro-mised mechanical property values of the original intact base material.

**2**

**M I C RO ST RU C T U R E A N D**

**M O D E L L I N G A P P ROAC H**

An actual composite microstructure is shown in Figure 1
where the MoSi2 particles, which is the discontinuous
phase, are randomly dispersed in the YSZ matrix. The
nominal volume fraction of the MoSi2 *particles is 20%.*
Additional information of the composite material such as
manufacturing process and details of the material
con-stituents of the composite can be found elsewhere.34 _{The}

geometry of the microstructure shown in Figure 1 was generated through postprocessing of an SEM image of the composite cross-section, which is then translated into a finite element mesh; see right side of Figure 1 showing a part of the mesh. A small initial precrack of length equal to 0.025 mm was included on the left side of the composite

specimen. The length and the width of the model are equal to 0.7 mm and 0.4 mm, respectively.

In the present work, cohesive elements are employed
for analysing fracture in the particle/matrix
sys-tem, whose behaviour is governed by the bilinear
traction-separation law.35 _{The microstructure is meshed}

using two-dimensional three-node plane-strain elements
(CPE3) for the particle and the matrix phases, to model
their bulk constitutive behaviour. In order to simulate
fracture, the initial finite element mesh was modified
using a Matlab pre-processing script to include four node
cohesive elements (COH2D4) throughout all the
interele-ment boundaries in the finite eleinterele-ment mesh. This process
of embedding cohesive elements throughout the mesh
introduces potential crack faces necessary to simulate
all the relevant fracture mechanisms such as interface
debonding, particle fracture, and matrix cracking.
How-ever, such an approach naturally triggers the issue of mesh
dependency in terms of the artificial compliance and the
converged crack path. This aspect has been taken into
con-sideration and subsequently resolved using the guidelines
derived from the mesh dependency study.16 _{The }

result-ing finite element mesh consists of about 106 _{elements,}
of which approximately 60% are cohesive elements and
the remaining 40% are plane-strain bulk elements. For
the bulk elements in the particle and the matrix phases,
a linear elastic and isotropic constitutive behaviour is
assumed. For the cohesive elements, the bilinear
cohe-sive relation (described below) is utilised, through which
corresponding fracture properties (strength and fracture
energy) are assigned for failure modelling in the particle,
the matrix, and the particle/matrix interface.

Note that the microstructure considered in the analysis is a cross-section of the particulate composite. Hence, the two-dimensional finite element model of the microstruc-ture does not entirely reproduce the microstructural

**FIGURE 1** Microstructure and loading conditions of a self-healing particle-matrix composite system. Finite element mesh was generated
after processing an SEM picture of (MoSi2) particles (lighter phase) embedded in yttria stabilised zirconia (YSZ, darker phase). A part of the

finite element mesh is shown on the right. Cohesive elements of zero geometric thickness were embedded along all interelement boundaries in the finite element mesh. A small initial precrack of length equal to 0.025 mm, schematically highlighted as a notch for better clarity, was included on the left side of the model. The length and the width of the specimen are equal to 0.7 mm and 0.4 mm, respectively [Colour figure can be viewed at wileyonlinelibrary.com]

**FIGURE 2** A bilinear traction-separation law, ie, with linear
softening. The arrows show steps such as loading, damage,
unloading, and reloading

features as the three-dimensionality is naturally lost in the model. As a matter of fact, the finite element model assumes that the cross-section of the particles is extruded in the third direction representing cylindrical inclusions rather than the actual particles. Despite these limitations, the microstructure-based fracture analysis in a two-dimensional framework is undertaken to reveal qualitative and some quantitative information in terms of the fracture mechanisms and the mechanical properties of the composites. Two-dimensional fracture analyses can be effectively used as a pragmatic approach to understand the effect of properties of the constituents (particle, matrix, and interface) on the crack path, a crucial information for self-healing material design.

For completeness and in order to introduce the required
notation, the cohesive zone model used in the present
anal-ysis is briefly summarised below.16,35,36 _{The cohesive law}

illustrated in Figure 2 corresponds to a bilinear relation
* between T, which is a scalar measure of the traction t*
transmitted across the cohesive surface, and Δ, which is a
scalar measure of the cohesive surface opening
displace-ment vector

*cohesive surface opening displacement Δ up to a maxi-mum value given by the material fracture strength,*

**𝜹. The traction T increases with increasing***𝜎*c, and eventually decreases linearly to zero, at which point the cohesive zone is fully separated. The area under the traction-separation curve, which represents the total work per unit area expended in creating a fully separated crack,

*corresponds to the fracture energy G*cof the material.

**The traction-separation law relates the traction t ***act-ing on the crack faces, with components (t*n*, t*s), to the
crack opening vector* 𝜹, with components (𝛿n, 𝛿*s), where
the subscripts “n” and “s” refer to the directions normal
and tangential to the crack face, respectively. An effective
crack opening Δ can be defined as

Δ ∶= √

*⟨𝛿*n⟩2+*𝛾*2*𝛿*s2*,* (1)

where ⟨·⟩ = (· + | · |) ∕2 refers to the Macaulay bracket
and*𝛾 is a non-dimensional mixed-mode parameter *
assign-ing weights for the modes I and II contributions, which is
defined as

*𝛾 =* *𝛿*n,0
*𝛿*s,0 *,*

where*𝛿*n,0and*𝛿*s,0denote, respectively, the crack opening
at the onset of failure for pure Mode-I and pure Mode-II.
*Denoting by tn,c* *and ts,c* the corresponding values of the
*normal and tangential cohesive strength, then tn,c* = *K𝛿n*,0
*and ts,c* = *𝛾*2*K𝛿*s,0. This will yield Δ0 = *𝛿*n,0 = *𝛾𝛿*s,0, and
*using the stiffnesses K and𝛾*2_{K}_{in modes I and II, }
respec-tively, then*𝜎*c = *t*n,c = *t*s,c∕*𝛾. Complete loss of cohesion*
occurs for pure modes I and II, respectively, at*𝛿*n,fand*𝛿*s,f,
with Δf = *𝛿*n,f = *𝛾𝛿*s,f.

In order to determine whether the crack opening is
increasing or decreasing due to the external loading
*pro-cess, the following loading function f*dis used:

*𝑓*d* _{= ̂}_{𝑓}*d

_{(Δ}

*d*

_{, 𝜅}_{) ∶= Δ −}

*d*

_{𝜅}

_{,}_{(2)}where

*𝜅*d

_{=}

*d*

_{𝜅}_{(}

_{t)}_{is a damage history variable that, at a}

*given time t, corresponds to the maximum value attained*by the equivalent crack opening during a process up to that time. The loading and unloading conditions correspond to the Karush-Kuhn-Tucker relations; see Figure 2.

The equivalent crack opening Δ is used to compute the
*equivalent traction T as*
*T = ̂T(Δ, 𝜅*d) =
{
*̂g(Δ)* if *𝑓*d_{=}* _{0 and ̇}_{𝜅}*d

_{> 0,}*̂g(𝜅*d

_{)}Δ

*𝜅*d otherwise

*,*(3)

where *̂g is the effective traction-separation law and ̇𝜅*d
indicates the (time) rate of change of the damage history
variable. The upper and lower expressions in (3) provide
the equivalent traction during, respectively, crack growth
and unloading/reloading. Alternatively, one could work
with a damage variable*𝜔 and consider a “damaged” *
stiff-ness such that (1−*𝜔)K = ̂g(𝜅*d_{)∕}* _{𝜅}*d

_{as indicated in Figure 2.}The specific form of the effective traction-separation law used in the present work is a linear softening relation (see Figure 2), which corresponds to

*g =* *̂g(Δ) = 𝜎*c⟨Δf− Δ⟩
Δf− Δ0

*.* (4)

The initially linearly “elastic” loading up to the fracture
strength in a bilinear law can be reproduced in Equation 3
by assigning an initial damage *𝜅*d_{(0) =} * _{𝜅}*d

0 = Δ0. The
parameter Δf *is chosen such that the integral of ̂T* from
Δ = 0 to Δ = Δf*equals the material fracture energy G*c,
i.e., Δf = *2G*c∕*𝜎*c.

After evaluating Equation 3, the normal and shear trac-tions can be computed as

*t*n=
{* _{𝛿}*
n
Δ

*T*if

*𝛿*n

*> 0,*

*K𝛿*n if

*𝛿*n

*< 0,*

*t*s=

*𝛾2 𝛿s*Δ

*T,*(5)

ie, for*𝛿*n **≥ 0, one has that t · 𝜹 = TΔ.**

The finite element model is subjected to a global Mode-I
loading by prescribing displacements on the upper and
lower edges of the specimen, which contains a small edge
precrack on the left as shown in the Figure 1. With
ref-erence to the literature,37,38_{the elastic properties used for}

the particle and the matrix are as follows: Young
*mod-ulus of the YSZ matrix is taken as E*m = 150 GPa and
that of the MoSi2*particle is given as E*p=450 GPa.
Pois-son's ratio of the particle and the matrix are kept equal
to 0.25. In the related literature, a significant scatter was
observed in the strength and the fracture energy of the
matrix and the particle and they depend on various
fac-tors such as temperature, manufacturing technique, and
chemical composition.39-42_{So, in the current study, a }

para-metric approach is taken, whereby a range of relative
fracture properties are considered and their effects on the
crack path and the composite properties are quantified.
The strength and the fracture energy of the matrix are
taken, respectively, as*𝜎*m

c =*300 MPa and G*mc =0.1 N/mm,
whereas the strength and fracture energy of the particle
and the interface (*𝜎*_{c}p*, G*p_{c},*𝜎*i

c*, G*ic) are varied with respect to
the corresponding matrix properties for the analyses. The
details on the fracture properties of the particle and the
interface and their variations are specified in the relevant
sections. All the analyses were conducted in Abaqus using
implicit Newton-Raphson iterative solver. A sufficiently
small value of viscosity equal to 1*.0 × 10*−6_{is used in the}
analysis to deal with convergence difficulties encountered
during the simulations, which involved multiple cracking
and coalescence in several cases.

The approach of the study is to conduct a series of parametric studies and to derive the composite specimen strength from the resulting load-displacement responses. It is to be noted that the term specimen (average) strength is used instead of effective strength, as the objective is not to derive homogenised composite properties, rather to reveal the role of fracture property mismatch on the global mechanical behaviour. The term “average” represents the normalisation of the load by the area over which the load is applied and the displacement by the corresponding length in the loading direction for the stress and the strain, respec-tively. However, the specimen properties obtained from the analysis would become the effective properties of the com-posite if appropriate measures are taken while applying the boundary conditions and if the specimen size is ensured

to be sufficiently large to be considered as a representative volume element (RVE). For convenience, the average spec-imen stress and the strain in the composite are denoted by

*𝜎*c_{and}* _{𝜀}*c

_{, respectively. The results obtained from this study}are presented in terms of normalised values of the above measures with respect to the corresponding values of the homogeneous (matrix) specimen.

In the next two sections, the effect of fracture prop-erties of the particle and the interface on the composite properties is investigated, for which a stiffer particle case is considered, by fixing the modulus mismatch ratio as

*E*p∕*E*m = 3, in accordance with the particulate composite
considered for the self-healing TBC.

**3**

**E F F EC T O F PA RT I C L E**

**F R AC T U R E P RO P E RT I E S O N**

**M EC H A N I C A L B E H AV I O U R**

The influence of the fracture properties of the particles on the specimen strength is analysed in this section. The variations in the crack path are reported for two repre-sentative cases, one corresponding to weaker particles and the second corresponding to stronger particles reinforced in the matrix material. Subsequently, a range of fracture properties (strength and energy) of the particles is consid-ered to study its effect on the mechanical response of the composite.

**3.1**

**Crack trajectory for particles**

**of different strengths**

**3.1.1**

**Weaker particle case**

A simulation is carried out with the properties mentioned in Section 2 for the particle and the matrix, except that the strength of the particle is reduced by 25% with respect to the matrix, resulting in a strength mismatch ratio,

*𝜎*p

c∕*𝜎*cm = 0*.75 between the particle and the matrix. The*
fracture energy of the particle and the matrix are kept the
same and equal to 0.1 N/mm. The particle is assumed to
be perfectly bonded to the matrix, which is achieved by
assigning a very high fracture strength for the interface
with respect to the properties of the particle and the matrix.
The simulated crack path through the microstructure is
shown in Figure 3 (indicated in white). It can be observed
that the propagating crack finds the weaker path by
frac-turing all the particles that are in the neighbourhood of the
advancing crack tip. In this case, particles fracture despite
the fact that the healing particles are stiffer than the matrix
by a factor of 3. Thus, the mismatch in the fracture strength
(making the particle weaker) has a stronger effect in
decid-ing the crack path when compared with the effect of the
mismatch in elastic properties. This result is relevant for

**FIGURE 3** Simulated crack growth on a particle/matrix system
with relatively weak particles given by the strength mismatch,
*𝜎*p

c∕*𝜎*cm=0*.75 between the particle and the matrix (propagating*

crack path is from left to right). Perfect particle/matrix bonding is
assumed in this simulation. A stiffer particle case is considered
*given by the elastic mismatch ratio, E*p_{∕}* _{E}*m

_{=}

_{3, between the}

particle and the matrix. The fracture energy of the particle, the matrix, and the interface are kept equal to 0.1 N/mm [Colour figure can be viewed at wileyonlinelibrary.com]

a capsule-based self-healing mechanism since it indicates that healing activation can be achieved even if the parti-cles are relatively stiffer than the matrix and crack-particle interaction is in principle deflective.

**3.1.2**

**Strong particle case**

The second case of interest is the situation when the
strength of the particle is higher than that of the matrix. In
this section, the simulation is performed with the material
properties indicated in Section 2, except that the strength
of the particle is increased by 25% as compared with the
matrix strength, which corresponds to a particle strength
mismatch ratio,*𝜎*cp∕*𝜎*cm =1*.25. The fracture energy of the*
particle and the matrix are kept the same and equal to
0.1 N/mm. Again, the bonding between the particle and
the matrix is assumed to be perfect. The resulting crack
path is reported in Figure 4 (indicated in white). From the
simulated crack path, it can be observed that the crack
propagates preferentially through the matrix, thus, in
gen-eral, avoiding the particles. However, on a few occasions,
particle fracture did occur, when the particle is directly in
front of the approaching crack. A similar observation has
been made in the literature.23 _{Such instances of particle}

fracture despite its higher strength can also be attributed to the irregular shape and clustering of the particles (ie, local stress conditions occur such that particle fracture is favoured). Furthermore, in these particular cases, pre-vention of particle fracture would require an unrealistic deflection of the crack tip. As a general conclusion, a composite with particles of higher strength precludes frac-turing of the particles. Such a scenario is unfavourable from a self-healing materials design viewpoint as this

**frac-FIGURE 4** Simulated crack growth on a particle/matrix system
with relatively strong particles given by the strength mismatch,
*𝜎*p

c∕*𝜎*mc =1*.25 (propagating crack path is from left to right). Perfect*

particle/matrix bonding is assumed in this simulation. Fracture energies of all the phases are kept the same and equal to 0.1 N/mm [Colour figure can be viewed at wileyonlinelibrary.com]

ture mechanism would prevent triggering of the healing mechanism.

**3.2**

**Effect on composite strength**

To analyse the effect of the fracture properties of the
parti-cles on the composite strength, a range of values of particle
strength ratios are considered, given by *𝜎*_{c}p∕*𝜎*cm = 0.05,
0.25, 0.33, 0.5, 0.75, 1, and 1.25. For each of the above
strength ratios, three different fracture energy ratios of the
particles with respect to the matrix fracture energy are
*con-sidered and are given by G*p_{c}∕*G*m

c=1/5, 1, and 5. The results of the simulations are summarised in Figures 5 and 6. Figure 5 shows the average stress-strain responses for some selected strength ratios, which provide the insights into the response history of the composite. Some important obser-vations can be made from the plot. Firstly, the strength of the composite specimen decreases with decrease in the particle strength. The strain corresponding to the peak stress (or strength) in the stress-strain curve decreases with decrease in the particle strength. It can also be noted that the point at which the curves deviate from the elastic response decreases as the strength decreases. This is an indication of the onset of damage prior to the peak load.

To summarise the results of all the simulations for vary-ing particle strength and fracture energy, Figure 6A shows the variation of the resulting strength of the composite specimen with respect to the particle fracture properties (strength and energy). As discussed before, the results clearly show a strong influence of the particle fracture properties on the mechanical response of the compos-ite specimen. From the plot shown in Figure 6A, it can be observed that decreasing the strength of the particle in relation to the matrix strength severely decreases the composite strength. For instance, the strength of the com-posite is decreased by 25% with respect to the reference

**FIGURE 5** Effect of particle strength on the normalised
stress-strain response of the composite specimen. The fracture
energy of the particle and the matrix are kept the same. Perfect
interface bonding is considered

homogeneous matrix specimen strength, when the parti-cle strength is reduced by 50%. On the other hand, increas-ing the particle strength above the matrix strength does not improve the strength of the composite as observed from the results. On the effect of fracture energy, a similar effect is i.e., decreasing the fracture energy of the particle reduces the composite strength as shown in Figure 6A. However, it has to be noticed that the effect of fracture energy ratio is pronounced only in the intermediate ranges of the strength ratios. In other words, when the particle strength is higher than that of the matrix or very low, then the composite strength is insensitive to the fracture energy of the particle as observed from the Figure 6A.

**3.3**

**Instances of particle fracture**

A parameter of interest for a particle-based self-healing
*mechanism is the percentage of fractured particles, p*
*which is defined as n∕N × 100, where n is number of*
*the fractured particles in the simulated crack path and N*
is the number of particles encountered or traversed by a
crack if the crack path were a perfect straight line
origi-nating from the initial crack tip. Through postprocessing
of the fractured microstructures for various particle
prop-erties, the percentage of fractured particles is determined
and plotted as the function of the fracture properties of the
particles in Figure 6B. As a general observation,
decreas-ing the strength of the particle favours particle fracture
as observed from Figure 6B, a requirement for healing
activation. However, the maximum number of fractured
particles saturates when the particle strength is reduced
below the strength ratio, *𝜎*_{c}p∕*𝜎*m

c = 0*.6, and is around*
160%. This indicates that the crack traverses the material

preferentially through particles located above and below
an ideal straight path. On the lower side, the percentage
of fractured particles reduces to just 10% if the particle
strength ratio is increased to a value beyond*𝜎*p_{c}∕*𝜎*m

c = 1. The fracture mechanism is very sensitive to the mismatch in the strength of the particle especially when the particle strength ratio is perturbed around the value of one.

When it comes to the fracture energy mismatch, the
effect is less pronounced as compared with the strength
ratio, which is consistent with the observations reported in
the previous work of the authors.16_{Increasing the fracture}

energy does not reduce the percentage of fractured parti-cles significantly, although reducing the fracture energy of the particle has a more pronounced effect as observed from Figure 6B.

The two plots showing the variation of the composite
strength and the percentage of fractured particles, with
respect to particle fracture properties provide an insight
on how to achieve a balance between the two
contra-dictory requirements for self-healing material design. For
instance, the objective of particle fracture (or healing
acti-vation) can be achieved with healing particles that are
only slightly weaker than the matrix. For example, for the
strength ratio,*𝜎*cp∕*𝜎*cm = 0*.833, a high percentage of *
frac-tured particles can be realised with just 5% reduction in
composite strength; see Figure 6B. Thus, if the healing
par-ticles can be engineered such that their strength is slightly
lower than the matrix strength, a successful self-healing
system can be achieved in terms of healing activation
without significantly compromising the fracture
proper-ties of the composite.

**4**

**E F F EC T O F I N T E R FAC E**

**F R AC T U R E P RO P E RT I E S O N**

**M EC H A N I C A L B E H AV I O U R**

Another important feature that governs the global mechanical behaviour of the particulate composite is the interface between the particle and the matrix. In the context of self-healing materials, the requirement on the interface properties is not straightforward. An ideal combination for a robust self-healing system would be a relatively weaker particle perfectly bonded to the surrounding matrix material. In that case, high inter-face strength is advantageous for efficient load transfer, whereby both the particles and the matrix are load-bearing constituents in the composite. However, if the particle is stronger than the matrix, particle fracture is less likely to occur, which, in turn, does not activate the healing mechanism when required. In such scenario, a relatively weaker interface could help in facilitating debonding between the particle and the matrix and expose the

heal-(A) (B)

**FIGURE 6** Effect of particle fracture properties on the composite strength and the percentage of fractured particles. The particle strength
is varied over a range, whereas for the particle fracture energy, three different ratios are considered as shown in the plots. A, Variation of
composite strength vs particle fracture properties. B, Normalised percentage of fractured particles vs particle fracture properties

ing particle to the crack. It is important to emphasise that
the term “interface” used here refers to a discrete zero
thickness layer between the particle and matrix with its
own fracture properties. In some practical cases,
encap-sulation of healing particles are done leading to a thin
third phase (interphase) layer between the particle and
the interface.14,43_{In such cases, the results obtained from}

the current study should be interpreted in the context that the failure of the interface would mean the failure of the encapsulating interphase layer.

To investigate the role of interface fracture properties, a series of simulations are conducted for varying inter-face fracture properties, while fixing the stiffness mis-match ratio between the particle and the matrix, given by

*E*p∕*E*m = 3. The strength and fracture energy of the
parti-cle and the matrix are kept the same and are given by*𝜎*p_{c} =

*𝜎*m

c = *300 MPa and G*

p

c = *G*mc = 0*.1 N/mm, respectively.*
Firstly, the crack path corresponding to a representative
system with a weak interface strength is discussed,
fol-lowed by detailed quantification of effect of the interface
properties on the mechanical response.

**4.1**

**Crack trajectory for an interface**

**of low bond strength**

The crack path resulting from the simulation with an
inter-face strength mismatch ratio,*𝜎*i

c∕*𝜎*cm = 0*.75, is shown in*
Figure 7. It can be observed that the crack predominantly
deflects its path towards the particle/matrix interfaces.
Crack advancement occurs primarily through debonding
along the interfaces between the particles and the matrix.
Nevertheless, at few instances, it is observed that particle
fracture occurs when the particle is directly in front of the
approaching crack or when it is relatively larger in size,
making it difficult for the crack to circumvent the
inter-face. From the perspective of successfully triggering the

**FIGURE 7** Simulated crack growth on a particle/matrix system
with relatively weak interface given by the strength mismatch,
*𝜎*i

c∕*𝜎*cm=0*.75 between the interface and the matrix (propagating*

crack path is from left to right). The fracture energy of all the phases are kept equal to 0.1 N/mm. The strength of the particle and the matrix are kept equal [Colour figure can be viewed at

wileyonlinelibrary.com]

healing mechanism, a weaker interface is in general not preferable as it does not necessarily lead to particle frac-ture. However, interface debonding could be considered as the second favourable fracture mechanism after particle fracture, as the probability of exposing the healing agent contained within the particle to the crack is likely to be high, potentially leading to healing activation.

**4.2**

**Effect on composite strength**

For detailed quantification of interface effects on the
mechanical behaviour, the average stress-strain responses
of the specimen with four different values for the
inter-face fracture strength,*𝜎*ic∕*𝜎*cm = 0*.01, 0.25, 0.5 and 1 are*
reported in Figure 8. From the figure, it can be seen that
an interface that is perfectly bonded (or at least having
equal fracture properties as that of the matrix and the
particle) results in a higher overall strength of the

**speci-FIGURE 8** Effect of interface strength on the normalised
stress-strain response of the composite specimen. The stiffness
*mismatch ratio is E*p_{∕}* _{E}*m

_{=}

_{3 that corresponds to a stiffer particle.}

Fracture strength of the matrix and the particle are kept the same.
The interface fracture energy is fixed and equal to that of the fracture
*energy of the particle and the matrix, G*i

c=*G*
p

c=*G*mc =0.1 N/mm

men as compared with the other responses corresponding
to lower interface strengths. This is an expected outcome
as stronger interface leads to better load transfer between
the matrix and the particle, resulting in higher strength.
However, it is worth noting that higher interface strength
or perfect bonding leads to a relatively brittle response in
the considered set-up. As the interface becomes weaker,
interface debonding is preferentially activated and
intro-duces an additional energy dissipating mechanism. This,
in turn, leads to enhanced energy dissipation and “ductile”
behaviour of the composite, albeit with a reduced
compos-ite strength. Such a scenario is often useful in composcompos-ite
materials with brittle-brittle phases whereby engineering
the interface aids in introducing ductility in the composite
material.44_{The term “ductility” is used in a general sense}

implying a non-abrupt fracture process and does not mean any plastic deformation. In the present context, it can be quantified as the ratio between the fracture strength and the fracture energy.

The results of several simulations are summarised in
Figure 8 in terms of the normalised stress as a function
of the strain for various values of the interface strength
and in Figure 9 in terms of the composite strength as a
function of interface strength and fracture energy. A clear
trend is observed revealing the improvement of the
com-posite strength with increase in the interface strength. The
strength of the composite specimen saturates when the
interface fracture strength is increased beyond the strength
of the particle and the matrix, as seen from the plateau
region of the curve in Figure 9 for*𝜎*i

c∕*𝜎*cm≥1 . On the other
end, when the interface strength ratio is reduced to a value

**FIGURE 9** Effect of interface strength and fracture energy on
strength of the composite specimen. The stiffness mismatch ratio is
*E*p_{∕}* _{E}*m

_{=}

_{3 that corresponds to a stiffer particle. Fracture properties}

of the matrix and the particle are kept the same

equal to 0.01 (interface strength is 100 times lower than that of the matrix and particle), the value of the compos-ite specimen strength reaches a lower limit approximately equal to 40% of the homogeneous matrix strength. This can be viewed as the strength of the composite with particles replaced by loose particles (or pores in the limit case) as the interface hardly plays any role in load transfer between the particle and the matrix. Such an explanation is appli-cable and valid only for tensile strength, but for the same composite under compression, the completely debonded particles would still contribute significantly to the load carrying capability through contact and frictional forces. On the effect of interface fracture energy, increasing the fracture energy of the interface by a factor of 5 does not significantly influence the strength of the composite, but decreasing the interface fracture energy by a factor of 5 reduces the composite strength as observed in Figure 9, which is a similar trend as seen in the effect of particle fracture energy in the previous section.

**4.3**

**Effect of mode-mixity on composite**

**strength**

While analysing fracture in composite materials (partic-ulate or fibre-reinforced), mixed-mode fracture is a com-mon phenomenon occurring in the failure of such mate-rials. Mixed-mode fracture arises from two main sources, one being the applied boundary or loading conditions in such a way that fracture evolves under globally applied mixed-mode loads. The second source is the inherent het-erogeneity of the material microstructure that leads to local mixed-mode fracture conditions in the vicinity of

the interfaces between the particles (or fibres) and matrix. This is often the case in composite materials, whereby even when the structure or the composite material is sub-jected to global Mode-I loading conditions, local stress fields in the crack vicinity are influenced by the presence of particles or fibres (and their interfaces), resulting in crack evolution under mixed-mode conditions. For many materials, the fracture properties are different for different modes of fracture (normal and tangential). More impor-tantly, the fracture properties of an interface between two material phases are found to be significantly different in opening (normal) and shearing (tangential) modes of frac-ture. Thus, it becomes a natural problem of significance to address the effect of varying interface fracture proper-ties in normal and tangential modes on the mechanical behaviour of the composite material.

In this subsection, fracture analyses are conducted
con-sidering different values of the interface strength in Mode-I
and Mode-II (normal and tangential strengths), and the
effects are quantified in terms of the resulting composite
strength. To this end, three sets of analysis are conducted
to address the above problem. Firstly, the interface
frac-ture strength (and the energy) is kept the same in both
modes (*𝛾 = 1). In the second set of analyses, the interface*
strength in Mode-II is taken equal to 10 times higher than
the strength in Mode-I (*𝛾 = 10, Mode-I dominated *
frac-ture). In the third set, the interface shear strength is reduced
by a factor of 5 as compared with its normal strength
(*𝛾 = 1∕5), enabling us to model an interface, which*
would easily yield to local Mode-II deformation field. In all
the three sets, the interface normal strength is varied over
a wide range, and the shear strength varies accordingly
in the three different sets of analyses described above.

The results of the simulations are obtained in terms
of the effective composite specimen response. The results
are summarised in Figure 10 in terms of the normalised
composite strength as a function of the interface strength
ratio, *𝜎*i

c∕*𝜎*cm, for three different values of mixed-mode
parameter, *𝛾. The ratio of the interface shear strength*
to the normal strength of the interface is specified by
the mix mode parameter *𝛾. From the results, it can be*
generally observed that increasing the shear strength of
the interface with respect to its normal strength (ie, with
increase in*𝛾) increases the resulting composite strength.*
For the mixed-mode parameter*𝛾 equal to 10 (higher shear*
strength), the composite strength is increased by
approx-imately 8% with respect to the baseline case (*𝛾 = 1) for*
most of the considered interface strength ratios. However,
once the interface (normal) strength is increased beyond
the matrix strength, the interface mixed-mode parameter
does not influence the composite strength. This is because
the interface debonding is automatically arrested when the
interface (normal) strength is higher than the matrix (and

**FIGURE 10** Effect of interface mixed-mode strength ratio on
strength of the composite specimen. Fracture properties of the
matrix and the particle are kept the same. The interface fracture
energies are kept equal to that of the fracture energy of the particle
*and the matrix, G*i

c=*G*pc=*G*mc=0.1 N/mm

particle) strength. Any further increase in shear strength of the interface with respect to its normal strength will not affect the strength of the composite.

On the other hand, for the mixed-mode parameter of
the interface equal to 0.2 (lower shear strength), the
influence on the composite strength is very strong as
observed from Figure 10. The resulting composite strength
is drastically reduced as compared with the strength in
Mode-I dominated case. This shows that though the
pre-scribed boundary condition is globally Mode-I loading,
local mixed-mode effects can play a significant role,
espe-cially if the strength of the interface is different in normal
and shear modes. In particular, the strength of the
com-posite under Mode-I loading is reduced by 30% for some
of the interface (normal) strength ratios considered.
Fur-ther, in the mixed-mode case with*𝛾 = 0.2, the reduced*
shear strength of interface affects the composite strength
even after the ratio of the interface strength ratio,*𝜎*i

c∕*𝜎*cm,
is increased beyond 1. From Figure 10, it can be observed
that saturation of the resulting composite strength occurs
only when the interface strength ratio is increased to
2.5 (or even above). Thus, the The mixed-mode fracture
properties can become important for composite behaviour
especially if the fracture properties are significantly
differ-ent in normal and tangdiffer-ential modes despite the loading
conditions being pure Mode-I or Mode-II.

**5**

**S U M M A RY A N D CO N C LU S I O N S**

In this study, micromechanical fracture simulations were conducted taking a real MoSi2 particle-filled TBC matrix

microstructure. The results obtained from the analyses reveal that the mismatch in fracture properties of the particle, the matrix, and the interface has a significant influence on the resulting crack path and the mechanical properties. From a self-healing viewpoint, the properties of the healing particle and the interface can be tailored to achieve the healing activation; however, on the other hand, such an approach affects the overall macroscopic strength of the resulting composite, which becomes detrimental to the material system. Care must be taken in order to achieve a trade-off between the resulting initial composite properties and the healing activation as it is natural that both the requirements could be contradicting in many practical self-healing materials. From the extensive fracture analyses on the composite microstructure, the following conclusions were arrived at:

**• The mechanical properties of the composite (the**

strength) are significantly influenced by the fracture properties of the particle. The effect of the particle strength is more pronounced than that of its fracture energy in determining the composite properties.

**• The percentage of fractured particles in the resulting**

crack path is very sensitive to the fracture strength of the particle. Particles that are slightly weaker than the matrix can trigger particle fracture (hence the healing mechanism), importantly without compromising the composite properties noticeably.

**• Interface fracture properties have a dominant effect**

on the composite properties. In case of interface-dominated fracture, mixed-mode fracture properties of the interface play a crucial role on the resulting compos-ite strength.

The results and conclusions from the microstructure-based crack propagation analyses can be used to get insights on pathways to achieve an optimal self-healing material system, ie, a design with the capability to trigger healing process but one which does not significantly lower the structural integrity of the original unfilled matrix material.

**AC K N OW L E D G M E N T S**

This work was funded in part by IOP Self-Healing Mate-rials (Agentschap NL, now Rijksdienst voor Onderne-mend Nederland RVO) through project SHM01021 and in part by the European Union's Seventh Framework Pro-gramme (FP7) through the NMP SAMBA project (grant number 309849). We thank the IOP Self-Healing Mate-rials and the Seventh European Framework Programme for their financial support of our research. We thank our collaborators Xun Zhang, Justyna Kulczyk-Malecka, and

Ping Xiao at University of Manchester for providing the microstructure. We extend our sincere thanks to our col-laborator Prof W. G. Sloof for his valuable support and interactive discussions.

**N O M E N C L AT U R E**

*T* effective traction

Δ effective opening displacement

* t* traction vector

* 𝜹* cohesive crack opening displacement vector

*t*n*, t*s cartesian components of traction vector
*𝛿*n*, 𝛿*s cartesian components of cohesive opening

displacement vector

*K* initial slope of cohesive law

*𝜎*c cohesive strength

*G*c fracture energy (toughness)

*E* Young's modulus of the material

*𝛾* non-dimensional mode mixity ratio

*f*_{d} loading function

*𝜅*d damage history variable

g effective traction-separation law

*𝜔* damage variable

Δ0 equivalent crack opening at onset of

damage

Δf equivalent crack opening at complete

failure

*𝛿*n,0*, 𝛿*s,0 crack opening at onset of damage for pure
mode I and mode II respectively

*t*n,c*, t*s,c cohesive strength for pure mode I and
mode II respectively

*𝛿*n,f*, 𝛿*s,f crack opening at complete failure for pure
mode I and mode II respectively

*𝜎*p

c*, 𝜎*cm*, 𝜎*ci cohesive (fracture) strength of particle,
matrix and interface respectively

*𝜎*p

c*, 𝜎*cm*, 𝜎*ci fracture energy (toughness) of particle,
matrix and interface respectively

*E*p*, E*m Young's modulus of particle and matrix
respectively

**𝝈****e** _{effective (or average) stress in the composite}

specimen

**𝝐****e** _{effective strain in the composite specimen}

*𝜎*m

c effective strength of a homogenous matrix

specimen

*𝜖*m

c effective strain corresponding to the

strength of a homogenous matrix specimen.

**O RC I D**

*Sathiskumar A. Ponnusami* http://orcid.org/
0000-0002-2143-8971

**R E F E R E N C E S**

*1. Bergman SD, Wudl F. Mendable polymers. J Mater Chem.*
2008;18(1):41-62.

2. Sloof WG, Pei R, McDonald SA, et al. Repeated crack healing in
MAX-phase ceramics revealed by 4D in situ synchrotron X-ray
*tomographic microscopy. Sci Rep. 2016;6(1):23040.*

3. Song GM, Pei YT, Sloof WG, Li SB, De Hosson JTM, van der Zwaag S. Oxidation-induced crack healing in Ti3AlC2ceramics.

*Scr Mater*. 2008;58(1):13-16.

4. Yıldırım G, Keskin ÖK, Keskin SB, ¸Sahmaran M, Lachemi
M. A review of intrinsic self-healing capability of engineered
cementitious composites: recovery of transport and mechanical
*properties. Constr Build Mater. 2015;101:10-21.*

5. Garcia SJ. Effect of polymer architecture on the intrinsic
*self-healing character of polymers. Eur Polym J. 2014;53:*
118-125.

6. Sloof WG, Turteltaub S, Carabat AL, Derelioglu Z, Ponnusami
SA, Song GM. Crack healing in yttria stabilized zirconia
ther-mal barrier coatings. In: van der Zwaag S, Brinkman E, eds.
*Self Healing Materials- Pioneering Research in the Netherlands*.
Netherlands: IOS Press; 2015:219-227.

7. Ono M, Nakao W, Takahashi K, Ando K. Strength recovery of machined Al2O3/SiC composite ceramics by crack healing.

*Fatigue Fract Eng Mater Struct*. 2007;30(12):1140-1148.
8. Pang JWC, Bond IP. ‘Bleeding composites’—damage detection

*and self-repair using a biomimetic approach. Compos Part A*
*Appl Sci Manuf*. 2005;36(2):183-188.

9. Yoshioka S, Boatemaa L, van der Zwaag S, Nakao W,
Sloof WG. On the use of TiC as high-temperature healing
*particles in alumina based composites. J Eur Ceram Soc.*
2016;36(16):4155-4162.

10. Kanellopoulos A, Giannaros P, Palmer D, Kerr A, Al-Tabbaa
A. Polymeric microcapsules with switchable mechanical
prop-erties for self-healing concrete: synthesis, characterisation and
*proof of concept. Smart Mater Struct. 2017;26(4):045025.*
11. Hilloulin B, Tittelboom KV, Gruyaert E, Belie ND, Loukili A.

*Design of polymeric capsules for self-healing concrete. Cement*
*Concrete Comp*. 2015;55:298-307.

12. White SR, Sottos NR, Geubelle PH, et al. Autonomic healing of
*polymer composites. Nature. 2001;409(6822):794-797.*

13. Kessler MR, Sottos NR, White SR. Self-healing structural
*com-posite materials. Compos Part A Appl Sci Manuf. 2003;34(8):*
743-753.

14. Carabat AL, van der Zwaag S, Sloof WG. Creating a protective shell for reactive MoSi2particles in high-temperature ceramics.

*J Am Ceram Soc*. 2015;98(8):2609-2616.

15. Kulczyk-Malecka J, Zhang X, Carr J, et al. Thermo-mechanical
properties of SPS produced thermal barrier coatings containing
pure and alloyed MoSi2 *particles. J Eur Ceram Soc. 2018;38:*

4268-4275.

16. Ponnusami SA, Turteltaub S, van der Zwaag S. Cohesive-zone
modelling of crack nucleation and propagation in particulate
*composites. Eng Fract Mech. 2015;149:170-190.*

17. Ayyar A, Chawla N. Microstructure-based modeling of the
influence of particle spatial distribution and fracture on
*crack growth in particle-reinforced composites. Acta Mater.*
2007;55(18):6064-6073.

18. Ayyar A, Chawla N. Microstructure-based modeling of crack
*growth in particle reinforced composites. Compos Sci Technol.*
2006;66(13):1980-1994.

19. Cannillo V, Manfredini T, Montorsi M, Siligardi C, Sola A.
Microstructure-based modelling and experimental investigation
of crack propagation in glass-alumina functionally graded
*mate-rials. J Eur Ceram Soc. 2006;26(15):3067-3073.*

20. Sozhamannan GG, Prabu SB, Paskaramoorthy R. Failures
analy-sis of particle reinforced metal matrix composites by
*microstruc-ture based models. Mater Des. 2010;31(8):3785-3790.*

21. Qing H, Liu T. Micromechanical analysis of SiC/Al metal matrix
*composites: finite element modeling and damage simulation. Int*
*J Appl Mech*. 2015;07(02):1550023.

22. Qing H. Micromechanical study of influence of interface
strength on mechanical properties of metal matrix composites
*under uniaxial and biaxial tensile loadings. Comput Mater Sci.*
2014;89:102-113.

23. Li Y, Zhou M. Prediction of fracture toughness of ceramic
com-posites as function of microstructure: I. Numerical simulations.
*J Mech Phys Solids*. 2013;61(2):472-488.

24. Li Y, Zhou M. Prediction of fractures toughness of ceramic
*com-posites as function of microstructure: II. Analytical model. J*
*Mech Phys Solids*. 2013;61(2):489-503.

25. Mishnaevsky L, Derrien K, Baptiste D. Effect of
microstruc-ture of particle reinforced composites on the damage
*evolu-tion: probabilistic and numerical analysis. Compos Sci Technol.*
2004;64(12):1805-1818.

26. Williams JJ, Segurado J, LLorca J, Chawla N. Three dimensional
(3D) microstructure-based modeling of interfacial decohesion in
*particle reinforced metal matrix composites. Mater Sci Eng A.*
2012;557:113-118.

27. Zhang J, Ouyang Q, Guo Q, et al. 3D Microstructure-based
finite element modeling of deformation and fracture of SiCp/Al
*composites. Compos Sci Technol. 2016;123:1-9.*

28. Gilabert FA, Garoz D, Paepegem WV. Macro- and
micro-modeling of crack propagation in encapsulation-based
self-healing materials: application of XFEM and cohesive
*surface techniques. Mater Des. 2017;130:459-478.*

29. Gilabert FA, Van Tittelboom K, Tsangouri E, Van
Hemel-rijck D, De Belie N, Van Paepegem W. Determination of
strength and debonding energy of a glass-concrete interface
*for encapsulation-based self-healing concrete. Cement Concrete*
*Comp*. 2017;79:76-93.

30. Quayum MS, Zhuang X, Rabczuk T. Computational model
*gen-eration and RVE design of self-healing concrete. Frontiers Struc*
*Civil Eng*. 2015;9(4):383-396.

31. Li W, Jiang Z, Yang Z, Yu H. Effective mechanical properties
*of self-healing cement matrices with microcapsules. Mater Des.*
2016;95:422-430.

32. Lv L-Y, Zhang H, Schlangen E, Yang Z, Xing F. Experimental
and numerical study of crack behaviour for capsule-based
*self-healing cementitious materials. Constr Build Mater.*
2017;156:219-229.

33. Wang L, Shao F, Zhong XH, et al. Tailoring of self-healing
*ther-mal barrier coatings via finite element method. Appl Surf Sci.*
2018;431:60-74. 5th Asian Conference on Heat Treatment and
Surface Engineering.

34. Kulczyk-Malecka J, Zhang X, Carr J, et al. Influence of embedded MoSi2 particles on the high temperature

ther-mal conductivity of SPS produced yttria-stabilised zirconia
*model thermal barrier coatings. Surf Coat Technol. 2016;308:*
31-39.

35. Ortiz M, Pandolfi A. Finite-deformation irreversible cohesive
*elements for three-dimensional crack-propagation analysis. Int*
*J Numer Meth Eng*. 1999;44(9):1267-1282.

36. Ponnusami SA, Krishnasamy J, Turteltaub S, van der Zwaag S.
A cohesive-zone crack healing model for self-healing materials.
*Int J Solids Struc*. 2018;134:249-263.

37. Schneibel JH, Sekhar JA. Microstructure and properties of
MoSi2-MoB and MoSi2-Mo5Si3*molybdenum silicides. Mater Sci*

38. Selçuk A, Atkinson A. Strength and toughness of tape-cast
*yttria-stabilized zirconia. J Am Ceram Soc. 2004;83(8):*
2029-2035.

39. Adams JW, Ruh R, Mazdiyasni KS. Young's modulus, flexural
strength, and fracture of yttria-stabilized zirconia versus
*temper-ature. J Am Ceram Soc. 2005;80(4):903-908.*

40. Kondoh J, Shiota H, Kawachi K, Nakatani T. Yttria
concentra-tion dependence of tensile strength in yttria-stabilized zirconia.
*J Alloy Compd*. 2004;365(1-2):253-258.

41. Schneibel JH, Kramer MJ, Ünal Ö, Wright RN. Processing and
mechanical properties of a molybdenum silicide with the
*com-position Mo-12Si-8.5B (at.%). Intermetallics. 2001;9(1):25-31.*
42. Petrovic JJ. Mechanical behavior of MoSi2and MoSi2

*compos-ites. Mater Sci Eng A. 1995;192-193:31-37.*

43. Ponnusami SA, Turteltaub S, Zhang X, Xiao P. Modelling crack
propagation in particle-dispersed self-healing thermal barrier
*coatings. In: van der Zwaag S, Brinkman E, eds. Self Healing*

*Materials- Pioneering Research in the Netherlands*. Netherlands:
IOS Press; 2015:229-241.

44. Yang J-M, Jeng SM. Interface and mechanical behavior of
MoSi2*-based composites. J Mater Res. 1991;6(03):505-513.*

**How to cite this article:** Ponnusami SA,
Krishnasamy J, Turteltaub S, van der Zwaag S. A
micromechanical fracture analysis to investigate the
effect of healing particles on the overall mechanical
response of a self-healing particulate composite.

*Fatigue Fract Eng Mater Struct*. 2019;42:533–545.
https://doi.org/10.1111/ffe.12929